# DOE Method of Concrete Mix Design | Concrete Mix Design by DOE Method

In this article, We’re going to create the DOE Method of Concrete Mix Design (Concrete Mix Design by DOE Method) with a concrete mix design example for a better explanation for making this concrete mix design calculation easy to understand so read the whole article download concrete mix design doe method pdf.

The civil Experience team works hard to provide the best guide for the Civil Engineering field so must follow us and share with friends if you gain valuable solutions from us.

## DOE Method of Concrete Mix Design

The DOE method was first introduced (published) in 1975 and then revised in 1988.

While Grading Curve Method was specifically developed for concrete pavements, the DOE method applies to concrete for most purposes, including roads.

Since the DOE method presently is the standard British method of concrete mix design, the procedure involved in this method is described instead of the outdated Road Note No 4 method.

### Step 1: Required Data for DOE Method of Concrete Mix Design

• Fineness modulus of selected F.A.
• Unit weight of dry rodded coarse aggregate.
• Sp. gravity of coarse and fine aggregates in SSD condition
• Absorption characteristics of both coarse and fine aggregates.
• The specific gravity of cement.

Let me take a concrete mix design example for data to make it easy to understand

1. Grade Designation = M 30
• For which we have to design concrete mix to achieve this particular strength of concrete for construction work of the project
2. Type of cement = O.P.C- 43 grade
• More than 17 different types of cement available for special construction work and every condition demand different material to more suitable, economical and durable structure.
3. Fine Aggregate = Zone-II
4. Sp. Gravity Cement = 3.15
5. Fine Aggregate = 2.61
6. Coarse Aggregate (20mm) = 2.65
7. Coarse Aggregate (10mm) = 2.66

### Step 2: Find Target Mean Strength

Find the target mean strength from the specified characteristic strength (Grade Designation)

Target mean strength = specified characteristic strength + (Standard deviation x risk factor)

Where risk factor is on the assumption that 5 percent of results are allowed to fall less than the specified characteristic strength.

Must need Excel Sheet for Civil Engineering and Structure design work. If you didn't download then you miss something important.

??=30+(1.65 ? 5.0)

??=38.25 ???

### Step 3: Calculate Water/cement ratio

Calculate the water/cement ratio. This is done in a rather round about method, using Table 11.11

Referring to Table 11.11, for OPC, uncrushed aggregate, for W/C ratio of 0.5, 28 days compressive strength is 49 MPa.

In the above Fig. find an intersection point for 42 MPa and 0.5 W/C ratios. Draw a dotted line curve parallel to the neighbouring curve. From this curve read off the W/C ratio for a target mean strength of 39 MPa.

The Water/cement ratio is = 0.58

Check this W/C ratio from durability consideration from Table 9.20. The maximum W/C ratio permitted is 0.50. Adopt lower of the two Therefore adopt a W/C ratio of 0.50

### Step 4: Calculation of Water Content

• Next, Decide the water content for the slump of 75 mm (assumed) 20 mm uncrushed aggregate from Table 11.12.
• In the case of CA & FA are different
• Water demand for natural fine aggregate = 195 lit
• Water demand for crushed coarse 20mm max size aggregate = 225 lit

????? ??????? = [(2/3)×W?]+[(1/3)×W??]

????? ??????? = [2/3×195]+[1/3×225]

????? ??????? = 205.0 ???3

Table 11.12: Approximate Free Water Contents Required to Give Various Levels of Workability According to the 1988 British method

### Step 5: Calculating Cement Content

Mixing water content is 205 kg/m3 of concrete.

?????? ??????? = 205/0.50

?????? ???????=410.0 ???3

Which is more than 350 kg (As per Table No. 9.2 of BS 8110: Part I: 1985) Hence o.k.

Also Read: What is the use of chicken wire mesh in construction Civil Experience

### Step 6: Calculating Weight of Total Aggregate

• This requires an estimate of the wet density of the fully compacted concrete. This can be found out in Fig. 11.4 for approximate water content and specific gravity of aggregate.
• Next, find out the density of fresh concrete from Fig. 11.4 for the water content of 205 kg/m3, 20 mm uncrushed aggregate of sp.gr. 2.65

The wet density = 2375.0 kgm3

The total weight of aggregate is found out for DOE Method of Concrete Mix Design

Weight of Total Aggregate = The wet density – (Weight of Cement + Weight of Free Water)

Weight of Total Aggregate = 2375 – (410 + 205)

Weight of Total Aggregate = 1760 kg/m3

### Step 7: Calculating Weight of Fine Aggregate

Then, the proportion of fine aggregate is determined in the total aggregate using below Fig. Fig. (a) is for 10 mm size, (b) is for 20 mm size and Fig. (c) is for 40 mm size coarse aggregate.

Also ReadConcrete Mix Design by IS, ACI and BS Methods: A Comparative Analysis

The parameters involved are the maximum size of coarse aggregate, the level of workability, the water/cement ratio, and the percentage of fine spassing 600 μ seive.

For 20 mm aggregate size, W/C ratio of 0.50, Slump of 75 mm, for 50% fines passing through 600 μ sieve, the percentage of

% ???? ????????? = 41 %

Weight of F.A. = 1760 × (41/100)

Weight of F.A. = 721.6 kg/m3

and

Weight of C.A. = 1760 × (59/100)

Weight of C.A. = 1038.4 kg/m3

### Step 8: Combination of Different Coarse Aggregate Fractions

Coarse aggregate can be further divided into different fractions depending on the shape of aggregate. As general guidance, the figures given in Table 11.14 can be used.

Also Read: How to Design Two Way Slab EXCEL Sheet by civil experience

### Step 9: Proportions for DOE Method of Concrete Mix Design

 Ingredients Quantity kg/m3 Ratio 1 Bag Cement Cement 410 1 50 Fine Aggregate 721.6 1.76 88 Coarse Aggregate 1038.4 2.54 127.0 Water 205 0.50 25 Chemical NM NM NM

### Step 10: Adjustment for Field Condition

The proportions are required to be adjusted for the field conditions. Fine Aggregate has surface moisture of 2 %

Weight of F.A. = 721.6 + (2/100) 721.6

Weight of F.A. = 736.03 kg/m3

Coarse Aggregate absorbs 1% of water

Weight of C.A. = 1038.4 – (1/100) 1038.4

Weight of C.A. = 1028 kg/m3

### Step 11: Final Design Proportions

 Ingredients Quantity kg/m3 Ratio 1 Bag Cement Cement 410 1 50 Fine Aggregate 728 1.80 90.0 Coarse Aggregate 1029.1 2.51 125.5 Water 205 0.50 25.0 Chemical NM NM NM
Also ReadConcrete Mix Design as per IS CODE easy way by excel sheet

Download DOE Method of Concrete Mix Design | Concrete Mix Design by DOE Method calculations pdf form Below

Download DOE method of concrete mix design example pdf from civil experience blog from below subscribe to unlock button and get doe method of concrete mix design example pdf file

FAQ 1:  Which Data Required for DOE Method of Concrete Mix Design?

1. Fineness modulus of selected F.A.2. Unit weight of dry rodded coarse aggregate.3. Sp. gravity of coarse and fine aggregates in SSD condition4. Absorption characteristics of both coarse and fine aggregates.5. Specific gravity of cement.

FAQ 2:  How to Find Target Mean Strength for DOE Method of Concrete Mix Design?

Find the target mean strength from the specified characteristic strength (Grade Designation) Target mean strength = specified characteristic strength + (Standard deviation x risk factor)Where risk factor is on the assumption that 5 percent of results are allowed to fall less than the specified characteristic strength.

The Civil Experiences always keep updating our Articles/posts with the latest civil engineering news, Structural Engineering Career tips, exam papers, Answer links Jobs & Information. So, Don’t forget to bookmark the Civil Experiences website and Please share this link with your friends to help them.